## electro-thermomechanical coupling of ferroelectric

## materials

Thesis by

### Vinamra Agrawal

In Partial Fulfillment of the Requirements for the

Degree of

Doctor of Philosophy

CALIFORNIA INSTITUTE OF TECHNOLOGY

Pasadena, California

2016

© 2016

Vinamra Agrawal ORCID: 0000-0002-1698-1371

### ACKNOWLEDGEMENTS

First, I would like to thank my advisor Prof. Kaushik Bhattacharya for his guidance,

support and many insightful discussions over the years. Prof. Bhattacharya has been

a great mentor. I learned a lot about doing research, choosing problems and asking

good questions. I am very thankful to Prof. Gurswami Ravichandran for being the chair of my thesis advisory committee and for many fruitful discussions throughout

the course of my graduate studies. I am also thankful to Prof. Ravichandran for his

guidance and advice at critical points of my career. I would like to thank Prof. Chris

Lynch for his useful insights on the behavior of ferroelectric materials, experimental

observations and challenges associated with conducting experiments on ferroelectric

materials. I would also like to thank Prof. Dennis Kochmann for always taking the

time to meet with me, giving valuable advice and feedback during the final years

of my graduate studies. I am very grateful to Prof. Nadia Lapusta for being on my

thesis committee and providing valuable feedback on my work.

Being a member of Prof. Bhattacharya’s group has been a great learning experience.

I especially enjoyed the joint Kaushik-Ravi group meetings and the discussions on

diverse topics such as mechanics of materials, pure and applied mathematics, applied

physics, experimental techniques and computational methods. I would like to thank

the past and present members of Prof. Bhattacharya and Prof. Ravichandran’s

research group: Mauricio Ponga, Likun Tan, Zubaer Hossain, Owen Kingstedt, Xin

(Cindy) Wang, Srivatsan Hulikal, Lincoln Collins, Dingyi Sun, Paul Plucinsky, Jin

Yang, Paul Mazur, Chun-Jen (Ren) Hsueh, Mike Rauls, Louisa Avellar and others for many helpful discussions, and for their support and friendship.

I had the privilege of becoming friends with many loving and exceptionally brilliant

people during my time at Caltech. I would like to thank Gaurav Sinha for his

friendship and our countless discussions over the years on mathematics, computer

science, physics, mechanics, politics, movies and other aspects of life. Along the

same lines, I would like to thank Vikas Trivedi for his friendship and support. I also

want to thank Likun Tan, Brandon Runnels, Xin (Cindy) Wang and Charles Wojnar for their friendship and valuable discussions over the years.

I was extremely fortunate to have become a part of the Los Angeles chapter of the

National Stuttering Association. I would like to thank Prof. Gail Lew who helped

the National Stuttering Association, past and current members of my chapter and

my friends John Gomez, Josh and Jen Marcus for their love and support.

Finally and most importantly, I am indebted to my parents and my brother for their

### ABSTRACT

How is material behavior at the macro scale influenced by its properties and

struc-ture at the micro and meso-scales? How do heterogeneities influence the properties

and the response of a material? How does nonlinear coupling of

electro-thermo-mechanical properties influence the behavior of a ferroelectric material? How can design at the micro-scale be exploited to obtain selective response? These questions

have been topics of significant interest in the materials and mechanics community.

Recently, new materials like multifunctional composites and metamaterials have

been developed, targeted at selective applications. These materials find applications

in areas like energy harvesting, damage mitigation, biomedical devices, and

vari-ous aerospace applications. The current thesis explores these questions with two

major thrusts: (i) internal reflects of shocks in composite media and (ii) shocks in

ferroelectric media.

Under the application of high-pressure, high strain rate loading, such as during high

velocity impact, shock waves are generated in the material. They can cause the

material to achieve very high stress states, and if transmitted without mitigation, can

lead to failure of key components. An important question here is ‘Can we design

materials which can successfully mitigate damage due to shocks?’ In a

heteroge-neous material, like a layered composite, the traveling waves undergo scattering

due to internal reflections. In order to understand internal reflections, an

ideal-ized problem that focuses on nonlinear shocks and ignores less important elastic

waves was formulated and studied in detail. The problem is studied by classifying all possible interactions in the material and then solving corresponding Riemann

problems. Using dynamic programming tools, a new algorithm is designed that

uses these solutions to generate a complete picture of the impact process. Different

laminate designs are explored to study optimal design, by varying individual layer

properties and their arrangement. Phenomena like spallation and delamination are

also investigated.

Upon high strain rate loading, ferroelectric materials like lead zirconate titanate (PZT) undergo ferroelectric to anti-ferroelectric phase transition leading to large

pulsed current output. These materials have thus found applications as pulsed power

generators. The problem of shock induced depolarization and the associated

electro-thermo-mechanical coupling of ferroelectric materials is studied in this thesis using

materials is conducted to study phase boundary propagation in the medium. The

presence of high electrical fields can lead to formation of charges in the material, such as surface charge on the phase boundary. Using conservation laws and the

second law of thermodynamics, a set of governing equations are formulated that

dictate the phase boundary propagation in isothermal and adiabatic environments.

Due to the possibility of surface charges on the phase boundary, the curvature of the

phase boundary starts to play a role in the driving force acting on the phase boundary.

The equations of motion and driving force see the contribution of nonlinear

electro-thermomechanical coupling in the material. Using the equations derived, a canonical

problem of impact on a ferroelectric material is studied. A new finite-volume,

### PUBLISHED CONTENT AND CONTRIBUTIONS

[1] Vinamra Agrawal and Kaushik Bhattacharya. “Impact induced depolariza-tion and electro-thermomechanical coupling of ferroelectric materials”. In: (2016). (To be submitted).

### TABLE OF CONTENTS

Acknowledgements . . . iii

Abstract . . . v

Published Content and Contributions . . . vii

Table of Contents . . . viii

List of Illustrations . . . ix

List of Tables . . . xiv

Chapter I: Introduction . . . 1

1.1 Shock waves in heterogeneous materials . . . 2

1.2 Shock waves and phase transitions . . . 4

1.3 Outline of thesis . . . 5

Chapter II: Fundamentals of shock waves . . . 7

2.1 Governing equations . . . 7

2.2 Plate impact . . . 8

2.3 Hugoniot curves . . . 10

2.4 Scattering and structured shock waves . . . 12

Chapter III: Shock wave scattering in layered materials . . . 21

3.1 Problem Description . . . 21

3.2 Governing equations . . . 22

3.3 Shock wave interaction at a material interface . . . 25

3.4 Semi-infinite medium . . . 28

3.5 Finite heterogeneous medium: Method . . . 28

3.6 Finite heterogeneous medium: Results . . . 37

3.7 Extensions and relaxing assumptions . . . 49

3.8 Conclusions and discussions . . . 51

Chapter IV: Pulsed power generation in ferroelectric medium . . . 55

4.1 Ferroelectric materials and pulsed power generation . . . 55

4.2 Continuum formulation . . . 61

4.3 Simplified one-dimensional analysis . . . 76

4.4 Shock wave propagation in ferroelectric materials . . . 78

4.5 Conclusions . . . 101

Chapter V: Summary and future directions . . . 104

### LIST OF ILLUSTRATIONS

*Number* *Page*

1.1 Different material response under different loading regimes. The

general domain for shock waves is shown inside the red circle. . . 2

1.2 Examples of heterogeneous materials. From left to right: concrete

core, polycrystalline steel and sand from Gobi desert . . . 3

2.1 Schematic of plate impact experimental setup. Flyer plate is launched

at high speeds through the launch tube. Particle velocity

measure-ments are done on the right end of the target through laser interferometry. 9 2.2 Schematic of shock transition states across a propagating shock. . . . 10

2.3 σ−ν Hugoniot for Aluminum 2024 alloy (material constants taken from [23]). The statesS+andS−are connected by a Rayleigh lineR.

The slope of the Rayleigh line can be used to obtain the speed of the

shock. . . 11

2.4 σ−vHugoniot for Aluminum 2024 alloy. . . 12 2.5 Us−v Hugoniot for Aluminum 2024 alloy. . . 13 2.6 (a) Shock waves are idealized as moving discontinuity. However,

a smooth, structured profile is observed (depicted in bold red) in experiments. The shock is preceded by an elastic precursor traveling

at speedUe. (b) Modifiedσ−Hugoniot curve to depict the Hugoniot Elastic Limit (HEL). The response is linear till σH E Lis achieved. . . 14 2.7 Schematic of the experimental setup used by Zhuang [89]. Particle

velocity profiles were captured for different combination of impact

speeds, layer thickness, material, layer arrangement and number of

layers. . . 15

2.8 (a) Variation of particle velocity profiles with impedance mismatch

in the periodic laminate. The impedance mismatch in PC74/Al37 is lesser than PC74/SS37, which means that shock is transmitted better

in PC74/Al37. As such the profile is steeper in this case. (b) Variation

of particle velocity profiles with number of interfaces in the laminate.

The profile with more interfaces has more ripples corresponding to

more scattering in the system. The profile steepens due to inherent

2.9 Schematic of the experimental setup used by Rauls [65]. A powder

gun accelerates an Aluminum impact to impact a two phase composite specimen. Measurements were done using PDV at the right end of

the target. . . 17

2.10 A cross section of the two phase composite sample used in [65] made from PMMA matrix and glass beads as inclusions . . . 18

2.11 Particle velocity profiles for bead size (a) 100µm and (b) 1000µm for 40% volume fraction. Profiles are measured at three points of the sample to account for spatial heterogeneity. The profile for 1000µm beads has less steep slope with rounded structures towards the leading and trailing edges of the shock. Additionally, the overshock is greater for the 100µm bead size due to greater number of beads, hence greater number of interfaces, leading to contributions from secondary reflections. . . 19

3.1 Schematic representation of plate impact . . . 22

3.2 (a) Illustration of elastic and shock waves in the stress-strain curve. The difference between the areas P3Q and P21 denotes the dissipation across the shock front. . . 24

3.3 (a) X −t diagram for the shock interaction problem at the A-B ma-terial interface. The impinging shockUAinteracts with the material interface to produce the elastic waves and a shockUB. . . 25

3.4 Schematic diagram of the elastic wave interaction at A-B interface . . 30

3.5 Elastic wave interaction leading to a compression shock . . . 31

3.6 Elastic wave interaction leading to an unloading shock . . . 31

3.7 Compression shock wave entering a purely elastic material . . . 32

3.8 Compression shock wave entering a purely elastic material . . . 32

3.9 Unloading shock wave entering another piecewise affine material . . 33

3.10 Interaction of elastic wave with compression shock . . . 34

3.11 Interaction of elastic wave and compression shock traveling in op-posite directions resulting in two possible solutions - (b) unloading shock wave and (c) compression shock wave. . . 34

3.15 Interaction of two elastic waves forming a compression shock in the

piecewise affine layer . . . 37 3.16 Interaction of two elastic waves forming a compression shock in the

piecewise affine layer . . . 37

3.17 Impact problem for L0 = 1m andεc decreasing linearly. (a) X −t

diagram of the impact problem. The red lines correspond to the

elastic waves while the black line is the propagating shock wave. (b)

Particle velocity profiles at X = 0 (left edge of the flyer), X = 1

(flyer-target interface) and X = 2 (right edge of the target). (c) Stress

profile at the flyer-target interface. The sudden drop in stress denotes

the arrival of the release wave from the free edge of the flyer. . . 39 3.18 Impact problem for L0 = 1m and εc increasing linearly. (a) X −t

diagram of the impact problem. (b) Particle velocity profiles atX =0

(left edge of the flyer),X =1 (flyer-target interface) andX =2 (right

edge of the target). (c) Stress profile at the flyer-target interface. The

sudden drop in stress denotes the arrival of the release wave from the

free edge of the flyer. . . 40

3.19 Variation of arrival times T with number of layers N for different

layer profiles . . . 41

3.20 Variation of particle velocity profile at the free edge of the target with

N for an alternate linear and nonlinear material. The first layer is chosen to be nonlinear with (a)ε2=0.2 and (b)εc =0.6. . . 42

3.21 Variation of particle velocity profiles with N for (a) linearly

de-creasing and (b) linearly inde-creasing εc profile. Profiles for constant εc =0.2, 0.6 are plotted for comparison. . . 44 3.22 Variation of particle velocity profiles with the exponent nfor (a) εc

decreasing and (b) εcincreasing profiles. . . 45 3.23 Variation of particle velocity profiles withλfor (a)εcdecreasing and

(b)εc increasing profiles. . . 46 3.24 Variation of particle velocity profiles withN for alternate layering of

(a)εc = 0.6 and 0.2 (b)εc =0.2 and 0.6. . . 47 3.25 X−tdiagram for the impact process on a layered target with (a)N =2

and (b) N = 20, where the εc increases linearly for both cases. A pair of tensile shocks is observed in both cases, with stronger shocks

3.26 Variation of total dissipation in the material with N for different εc arrangement. The flyer length is chosen to be large to avoid the effect of release waves. The dissipation is higher for the layer arrangement

withεc decreasing linearly along the length. . . 49 3.27 Potential solutions for initial impact on a layered composite with

the modified piecewise affine stress-strain curve. For small impact

speeds, the maximal dissipation kinetics ensures (a), (b) a two wave

structure. For high impact speeds (c), (d) a single shock wave is

sufficient for a unique solution. . . 50

4.1 Characteristic curve of a ferroelectric material. At zero electric field,

the material exhibits a non-zero polarization (≈ 33µC/cm2 in this case). . . 56

4.2 (a) Experimental setup for loading a PZT sample hydrostatically, and

measuring D − E loops. (b) Variation in the characteristic curve of a ferroelectric material upon application of hydrostatic pressure

(Figures from [78]). . . 57

4.3 Schematic of ferroelectric generators providing shock loading to the

material through (a) plate impact and (b) blast loading . . . 58

4.4 (a) Schematic of the experimental setup used by Furnish et al. [34].

(b) Charge profiles obtained through the external circuit. The num-bers on top of the individual profiles denote different experimental

runs. Parameters for each experimental run are available in [34]. . . . 60

4.5 Continuum representation of the problem. The material is subjected

to a generalized electromechanical loading in the deformed frame. A

phase boundary propagates causing FE-AFE phase transition. . . 61

4.6 Schematic of the canonical uniaxial impact problem. A phase

bound-ary propagates in a one dimensional system after being impacted by

a flyer. The two ends of the ferroelectric material are connected

through a resistor R. Current flowing through Ris tracked. . . 79 4.7 (a) Hε energy landscape of the ferroelectric material. The

en-ergy wells change based on temperature, but εT is unchanged. (b) Schematic of Cauchy stress σcprofile for the ferroelectric material. . 81 4.8 (a) Riemann problem at the node ˜xiother than at a phase boundary or

at either of the ends of the material. The problem is solved keeping the

temperature constant. (b) Temperature update at the node following

4.9 (a) Riemann problem to be solved at the phase boundary. The speed

of the phase boundary is also unknown. This is where the kinetic relation comes into equation. (b) Temperature update at the phase

boundary. . . 87

4.10 (a) Conservation of momentum problem at the flyer target interface.

(b) Temperature update using the conservation of energy equations. . 89

4.11 Schematic of the mesh update procedure [64]. As the phase boundary

gets closer to a node, the node is removed and the mesh is resized.

Once the phase boundary gets further away, the node is reinserted. . . 90

4.12 (a) Linear kinetic relation. (b) X −t diagram of the impact problem. The colors correspond to the strain in the flyer and the ferroelectric target. The speed of the impact is 75 m/s. . . 93

4.13 (a) Current profile obtained flowing through the resistorRfor an

im-pact speed of 75 ms−1. (b)X−tdiagram of the impact problem. The colors correspond to the temperature in the flyer and the ferroelectric

target. . . 94

4.14 (a) Variation of current profile with increasing impact speeds. (b)

Variation of current profiles with changing values of ds for impact

speed of 75 m/s. . . 95

4.15 (a) Variation of current profile with increasing impact speeds. (b) Variation of current profiles with changing values of ds for impact

speed of 75 m/s. . . 96

4.16 Variation of current profiles withRin the external circuit for the same

impact speed 75 ms−1. . . 96 4.17 (a) Combination of Stick-slip and Linear kinetic relation. (b) X −t

diagram of the impact problem. The colors correspond to the strain

in the flyer and the ferroelectric target. The speed of the impact is

75 m/s. . . 97

4.18 (a) Comparison of current profiles for Linear and Stick-Slip Linear Kinetic relation. (b)X−tdiagram of the impact problem. The colors correspond to the temperature in the flyer and the ferroelectric target. 98

4.19 (a) Stick-exponential slip kinetic relation (b) Comparison of charge

profiles from experiments and simulations . . . 100

4.20 Shock speed vs Particle speed Hugoniot of the ferroelectric material

for different R in the external circuit. The figure shows a clear

### LIST OF TABLES

*Number* *Page*

4.1 Choice of ferroelectric material parameters . . . 91

4.2 Choice of flyer material parameters . . . 91

4.3 Choice of parameters in setting up the problem . . . 91

4.4 Setup and material parameters in experiments by Furnish [34] . . . . 99 4.5 Choice of material and setup parameters for simulations . . . 99

4.6 Variation of Hugoniot parameters of the ferroelectric material for

different values of Rin the external circuit. The Hugoniot, and hence

the material behavior, shows strong dependence on the external circuit

*C h a p t e r 1*

### INTRODUCTION

High velocity impacts are very common in nature as well as day to day life. For

example, in an automobile accident, the structural elements of the vehicle undergo

very rapid loading and large deformations. The impact speed involved, in an

extreme case, is around 60 ms−1 with pressures reaching up to 1 GPa in a time frame of a few milliseconds. Another very important scenario is that of a bird

strike on an airplane. In this case, the impact happens at speeds of the order of 100 ms−1, and can cause tremendous damage to life and property. Moving towards military and defense scenarios, the pressure and time scales involved can be orders

of magnitude different. A ballistic impact or a blast loading involve loading speeds

up to 1−5 kms−1and 6−10 kms−1with pressure increase ranging from 1−10 GPa within a few microseconds. The pressure increase and impact speeds typically

increase as the applications move away from earth and into space. Orbital debris

is present at various altitudes, with sizes ranging from 1−10cm. The debris can achieve speeds greater than 10 kms−1. Dealing with orbital debris has proven to be a major challenge, and many objects of size larger than 5 cm are tracked to avoid any possible collisions. Impact involving small astronomical objects, such as small

meteorites, can happen at speeds of up to 10 kms−1, while an impact involving larger astronomical objects can happen at speeds of up to 20−50 kms−1.

High velocity impact leads to high pressures and high strain rates, and this in turn can

lead to shock waves. Figure 1.1 shows a schematic of different material responses

over a range of applied pressure and strain rate loading. The loading regime for

shock behavior is circled in red. Under shock loading, the material experiences

extreme environments undergoing large temperature and pressure changes over a very short period of time. If these waves are left to travel unmitigated, they can

cause significant damage in the material.

Due to such broad applications, understanding material behavior in high strain rate

conditions is very important. Studies pertaining to shock waves in solids started

during the early 1900s, and generated significant interest during the 1940s and 1950s

because of numerous military applications. In order to characterize and predict

Figure 1.1: Different material response under different loading regimes. The general domain for shock waves is shown inside the red circle.

and numerical investigations have been undertaken. Over the years, the focus of

investigation has expanded from metals and metallic alloys to ceramics, polymers,

composites and even soft materials. Further, the focus has also expanded from

studying just wave interactions to understanding shock induced chemical changes,

phase transformations, metallurgical defects and fragmentation.

**1.1** **Shock waves in heterogeneous materials**

Heterogeneous materials cover a broad spectrum of materials such as composites, polycrystalline materials, polymers, etc. In fact, except for perfect single crystals,

every material is heterogeneous at some length scale. Composite materials are now

widely used due to their superior effective properties over their constitutive

materi-als. For example, concrete - a two phase composite with matrix and inclusions - is

a common structural material with high compression strength and low thermal

ex-pansion coefficient. Kevlar is another such example of a composite which has found

wide applications ranging from armors to durable tires because of its high

tensile-strength-to-weight ratio. Polycrystalline materials like steel have found applications

in automotive and structural industries due to their broad range of yield stress and elastic modulus depending on different manufacturing processes. The

manufactur-ing processes essentially control the microstructure such as grain size and orientation

in the material. Sand is another class of heterogeneous materials with many

dif-ferent compositions, granular structures and grain distributions depending upon the

Figure 1.2: Examples of heterogeneous materials. From left to right: concrete core, polycrystalline steel and sand from Gobi desert

defense to agriculture and construction.

Due to such widespread applications, it is important to understand shock behavior

of heterogeneous materials and the role of heterogeneity in the response. Wave

propagation in heterogeneous materials has been a topic of interest in the community

for many decades. Most of the work in the early years had been focused on wave

dispersion of small amplitude waves in linear elastic periodic materials [74], [61].

Experiments conducted by Barker and others [13] on periodic laminates showed

exponential decay of stress waves with distance to achieve a structured steady

profile above a critical stress amplitude. Other experiments [50], [63] on layered materials show resonance phenomena. In recent years, many shock studies have

been conducted on heterogeneous materials to understand the role of heterogeneity

(see [29], [65], [80], [81], [89] and references therein).

Much less is known regarding the theoretical side of shock wave propagation in

heterogeneous materials. The formation of structured shock waves was studied

extensively in homogeneous metals ([75], [58]) and the primary mechanism was

attributed to viscoelastic and viscoplastic behavior of these materials. These

theo-retical models worked very well in predicting the steady shock width in metals. For

heterogeneous materials, Grady [35] presented scattering of nonlinear waves as an

alternate explanation for structured waves. The complexity of the physics behind

wave propagation in a heterogeneous material can be illustrated by looking at the interplay between the length scale of heterogeneity and the shock width and the

associated response. The following equation

ρ(x)utt =

σ ux, x h x

−γ
_{x}

h

ux x x x+ν

_{x}

h

ux xt, (1.1) represents a one-dimensional augmented wave equation for a heterogeneous material

and coefficient of viscosity of the material. It can be seen from the above equation

that there are two length scales in the problem - size of the heterogeneity h and the width of the wave l = pγ/ρ. The asymptotic behavior can be summarized as follows:

1. l h: In this case, the wave width is much larger than the size of the heterogeneity. As such, the wave sees an effective environment as it propagates

through the medium [76].

2. l h: In this case, the wave width is much smaller than the sixe of the heterogeneity. Here, as the wave propagates, it sees material interfaces and

different material environments across the interface and reacts accordingly. Here the motion is dominated by reflections and scattering.

In the first half of this thesis the phenomena of scattering (l h) of shock waves is explored. A canonical problem of plate impact on a layered, not necessarily periodic, material is taken into consideration. The layered material is impacted

upon by a flyer traveling at high speed. The fundamental problems such as

wave-wave interaction and wave-wave-interface interaction are studied to develop an overall

picture of shock wave propagation.

**1.2** **Shock waves and phase transitions**

Under shock loading, the ground state of a material can be driven from one energy

minimum to another, resulting in dynamic crystal reorientation over a short period

of time. The process of shock induced phase transitions in metals has been

exten-sively studied, including nucleation and kinetics (see [56], [28], [8], [33], [43] and

references therein). In case of special materials like ferroelectric and ferromagnetic materials, characterized by a strong nonlinear electro-magneto-thermomechanical

coupling, shock loading can induce electrical or magnetic phase transitions. This

phase transition is accompanied by large pulse of power under certain

electromag-netic boundary conditions. As such, these materials have found applications as

pulsed power generators [7]. In this thesis the focus will be placed on ferroelectric

materials. It should be noted that, at a continuum level, the analysis for ferromagnetic

materials proceeds in a similar fashion.

Experimental investigations into the dynamic loading behavior of ferroelectric

ma-terials date back to 1959 [14]. Since then many experimental studies have been

the shock response of these materials under different configurations and boundary

conditions. Plate impact experiments have been a standard method for these exper-iments due to their ease of setup and control over various parameters. Almost all

studies are conducted on either axially poled, normally poled or unpoled samples.

The poling configuration corresponds to the alignment of polarization direction

with the direction of loading. It has also been found that behavior is different under

short-circuit and open-circuit boundary conditions. Further, experiments have been

conducted for different compositions of Lead Zirconate Titanate (PZT) specimens,

and it has been found that PZT 95/5 doped with 2% Niobium can be depolarized at

low shock speeds.

While there are many experimental studies, relatively less is known about the

the-oretical aspects of shock induced phase transitions and power generation. In this

thesis, the theoretical aspects of shock induced phase transitions in a ferroelectric

material are studied.

**1.3** **Outline of thesis**

This work is organized as follows. Chapter 2 covers the fundamentals of shock

wave propagation. A detailed derivation of governing equations for the motion of

a jump surface (across which quantities like deformation gradient, traction, particle

velocity, etc. are discontinuous) is presented. A brief introduction and description

of the standard plate impact experiment is provided along with the simplification it brings to the analysis. The idea of Hugoniot curves is introduced next and the

well known linear shock speed - particle speed relationship is discussed. Finally,

a detailed discussion on scattering and the formation of structured shock waves is

presented.

Chapter 3 deals with a canonical problem of a plate impact on a model layered, not

necessarily periodic, material. In order to deal with only Riemann problems, the

Hugoniot is approximated by a piecewise linear stress-strain curve. A maximally

dissipative kinetic relation is introduced to obtain a unique solution. This can also be seen as an equivalent relation to Lax entropy criteria in shocks. The complex

wave problem is broken down into classes of fundamental interactions and analytical

solutions are obtained for each of these classes. These solutions are then stitched

together to obtain a complete picture of the wave propagation. Next, a broad

parameter study is conducted to study the influence of material interfaces, layer

made on the optimal design of a material for shock attentuation.

In chapter 4, shock wave propagation in a ferroelectric material is studied.

Fer-roelectric materials under shock loading undergo ferFer-roelectric to antiferFer-roelectric

phase transition to produce a large pulsed power output. The nonlinear

electro-thermomechanical coupling of ferroelectric material plays a central role in this

process. A continuum analysis for large deformation dynamic behavior of a

fer-roelectric material is presented. Governing equations as well as an expression for

driving force acting on the phase boundary are derived using conservation laws,

Maxwell equations and the second law of thermodynamics. Next, the canonical problem of plate impact on a ferroelectric material is studied. Numerical

simu-lations are conducted to study the current output through the resistance R in the

external circuit. Finally current profiles are compared with experiments and the

shock-speed particle-speed Hugoniot of the material is generated for short and open

*C h a p t e r 2*

### FUNDAMENTALS OF SHOCK WAVES

In this chapter, the basic theory behind shock waves will be presented, which will

be useful in subsequent chapters. For detailed derivations and interpretation the

reader is directed to [23] and [10] and the references therein. Ideally, shock waves are characterized as a moving discontinuity of stresses, strains, density, particle

velocity, temperature, etc.

**2.1** **Governing equations**

In this section, equations and jump conditions that govern the motion of a body

under large dynamic deformation with a propagating phase boundary are derived.

For reference, this derivation can be found in [2].

Consider a deformation map**y**(**x,**t)mapping a bodyBin its reference configuration
to its deformed configuration. The body also contains a propagating regular surface

S0(t)across which different quantities might be discontinuous. This map is assumed

to be continuous everywhere, but first and second derivatives can be discontinuous.

The deformation gradient**F**and particle velocity are defined as**F**(**x,**t)= Grad**y**(**x,**t)

and**v**(**x,**t) = ∂y(**x,**t)/∂t, where**x**refers to the coordinates in the reference frame.
At any given point**x**in the reference frame, let ρ(**x**) denote the density,**b**(**x,**t) be
the body force per unit mass andσ(**x,**t)be the nominal stress tensor. The integral
form of conservation of linear and angular momentum in any arbitrary subdomain

D ⊂ Bcan be written as

Z

∂D

σ**n**ˆ dA+

Z

D

ρbdV = d dt

Z

D

ρvdV, (2.1)

Z

∂D

**y**×σ**n**ˆ dA+

Z

D

**y**× ρbdV = d
dt

Z

D

**y**× ρvdV. (2.2)
Further, the conservation of energy for the arbitrary subdomainDcan be written as

Z

∂D

σ**n**ˆ·**v**dA+

Z

D

ρb·**v**dV+

Z

∂D

**q**·**n**ˆdA+

Z

D

ρr dV = d

dt

Z

D

ρε+ 1

2ρv·**v**

!

dV,

(2.3)

production as,

ΓD(t) B d dt

Z

D

ρηdV − Z

∂D

(**q**·**n/θ**ˆ )dA−
Z

D

ρr/θdV. (2.4)

Here, θ is assumed continuous with piecewise continuous derivatives and η is piecewise continuous with piecewise continuous derivatives. The Clausius-Duhem

inequality for arbitraryD ⊂ Band for all timetenforces

ΓD(t) ≥ 0. (2.5)

Next, Coleman-Noll type arguments can be implemented to localize the above equations to get following equations at any point not onS(t).

Divσ+ ρb= ρ**v,**˙ (2.6)

σFT _{=} ** _{Fσ}**T

_{,}

(2.7)
σ·**F**˙ +Div**q**+ ρr = ρε,˙ (2.8)

Div(**q/θ**)+ ρr/θ ≤ ρη.˙ (2.9)

Additionally, at any point onS(t)the following jump equations can be obtained:

~σ**n**ˆ+ ρVn~**v**= 0, (2.10)

~σ**n**ˆ ·**v**+~ρ(ε+**v**·**v/2**)Vn+~**q**·**n**ˆ=0, (2.11)

~**q**·**n/θ**ˆ +~ρηVn ≤ 0, (2.12)

where~·denotes the jump in quantities across the surfaceS(t). Further,Vn =**V**·**n**ˆ
is the normal velocity ofS(t), conventionally taken to be positive in the direction of

the normal.

In addition to the above equations, certain kinematic compatibility equations are

enforced across S(t) to ensure continuity of **y. Let ˆt**be the tangent vector at any

pointS(t). The compatibility equations are given by

~**F**ˆ**t**= 0, (2.13)

~**v**+Vn~**F****n**ˆ =0. (2.14)

**2.2** **Plate impact**

The plate impact experiment is the most common and widely used method to

investigate shock propagation in a material. The experiment involves accelerating a

are circular disks of very small thickness compared to their diameter. Measures are

taken to ensure that the plates have smooth surfaces. This ensures that the impact is uniform and the momentum is transferred evenly to the target surface. Typical

target thickness ranges from 1 mm to 1 inch. A typical setup for the plate impact

experiment is represented in Figure 2.1.

Figure 2.1: Schematic of plate impact experimental setup. Flyer plate is launched at high speeds through the launch tube. Particle velocity measurements are done on the right end of the target through laser interferometry.

Plate impact experiments are designed to produce uniaxial loading conditions from

the moment of impact until the release wave from the left end (and typically the

free end) of the flyer. Since shock experiments happen at very short time scales,

there is no time for the system to exchange heat. This makes the plate impact

experiments adiabatic. Further, there are no external volumetric heat sources. This
means**q**= 0 andr = 0. As such, the jump equations from Section 2.1 reduce to a

set of one-dimensional equations as below:

~σ+ ρ0Us~v= 0, (2.15) ~v+Us~= 0, (2.16) ~σv+ ρ0Us~ε+v2/2= 0, (2.17) where ρ0, , σ andUs denote the reference density, uniaxial strain, uniaxial stress

and the speed of the propagating shock. The schematic for shock transition states is represented by Figure 2.2. The statesS− andS+ represent the state of the material

before and after the shock wave has propagated. Typically the target is at rest in a

Figure 2.2: Schematic of shock transition states across a propagating shock.

**2.3** **Hugoniot curves**

Shock jump equations (2.15)-(2.17) are not enough to completely determine the final

states and the speed of the shock. Further, the equations do not contain material

information to distinguish one material from another. If the state S− in Figure 2.2

is kept fixed and stronger shocks are introduced in the system, a locus of states

S+ can be generated. This locus is called a *Hugoniot* centered around S−. The

Hugoniot, a characteristic curve of a material, contains the minimum amount of

information required to solve the shock propagation problem to obtain the final state

S+. However, the Hugoniot curves do not provide the complete thermodynamical material description. This is where an equation of state (EOS) is needed. An EOS

is a comprehensive material model that takes various thermodynamic parameters

into account. As such, Hugoniot relations can be obtained from an EOS after

mechanical and thermodynamical analysis. For a detailed review on various EOS

and their analysis, the reader is referred to [23].

Given an initial state, the S+ states σ, , v, ε and Us together form 10 pairs of
Hugoniot. In case of zero initial particle velocity and stress free state, the Hugoniot
is called a*principal Hugoniot*curve. Using an EOS, Hugoniot centered around other

initial states can also be determined. Due to ease of measurement, specific volume νis measured instead of strain. Among these, the mostly commonly used Hugoniot curves are σ − ν, σ − v andUs − v curves. The σ − ν curve provides valuable thermodynamic information about the material, theσ −v relation provides direct measurements of stresses given particle velocity profiles obtained from experiments,

and theUs−vrelation enables direct measurement of propagating shock speed.

relation can be obtained from this by using =1−(ν/ν0), whereν0is the reference

specific volume given by ν0 = 1/ρ0. The line R connecting the states S− and S+

is called the Rayleigh line, the slope of which related to the speed of the shockUs.

This means that a faster shock would lead to steeper R and consequently higher

stress states. Further, using (2.17), it can be shown that the area under the Rayleigh

line in Figure 2.3 denotes the jump in specific internal energy of the material during

the shock.

Figure 2.3: σ−νHugoniot for Aluminum 2024 alloy (material constants taken from [23]). The states S+ and S− are connected by a Rayleigh line R. The slope of the Rayleigh line can be used to obtain the speed of the shock.

Figure 2.4 shows theσ−vHugoniot curve for Aluminum 2024 alloy corresponding to the shock propagating in the +x direction. This curve is becomes very useful while solving impact problems to directly obtain stress states. One of the most

common observations of plate impact experiments is that the velocity of the shock is

proportional to the particle velocity of the material upon impact. This observation is

consistent with many solids over a wide range of impact speeds. These experiments

are typically conducted at room temperature (∼ 300K) on unstressed sample with zero initial particle velocity. The linear law is given by

Us =C+Sv+, (2.18)

whereCandSare material constants computed from the experiments. Typically,C

is found to be close to the bulk sound speed in the material. Sis a dimensionless

con-stant which typically ranges from 1-2 for most materials. A list of Hugoniot curves

Figure 2.4: σ−v Hugoniot for Aluminum 2024 alloy.

(2.18) into the jump equations (2.15) and (2.16) with reference initial conditions,

we get

σ+ = (ρ0C)2(ν0−ν+)

1− ρ_{0}S(ν0−ν+)2

, (2.19)

σ+ _{=} _{ρ}

0(C+Sv+)v+. (2.20)

Figure 2.5 shows theUs−vHugoniot of Aluminum 2024 alloy, where they-intercept corresponds toC. For Aluminum 2024, following values were used [55]

ρ0 =2785 kgm−3, C =5328 ms−1, S=1.338. (2.21)

**2.4** **Scattering and structured shock waves**

Although shock waves are ideally characterized as moving discontinuities, it has

been observed that they have a structure. The stress states, instead of being discon-tinuous, vary smoothly and sharply over a small region connectingS+ andS−. This

is represented in Figure 2.6a by∆x. Further, the shock wave is preceded by an elastic

precursor traveling at speedUe. This means the Hugoniot response doesn’t kick in

until a threshold state is achieved. Formally this means that the σ −ν Hugoniot curve is preceded by a linear relation which is valid up to a certain limit as shown in

Figure 2.6b. This is called the Hugoniot Elastic Limit (HEL) of the material [23].

Figure 2.5: Us−vHugoniot for Aluminum 2024 alloy.

The processes behind the formation of a structured shock wave has been a matter

of extensive research. This is because shock attenuation can not only be achieved

by lowering the stress σ+, but also by increasing the rise time of the pulse. The formation of a structured shock wave has traditionally been attributed to inelastic

processes, such as viscoelasticity [11], viscoplasticity ([9], [41], [75]) and twinning. Swegle and Grady [75] conducted shock impact studies on eight different materials,

six metals and two insulating solids. They observed a power law scaling between

the peak strain rate in the shock and change in stresses across the shock front,

˙

= β(∆σ)hSG_{, where}_{hSG} =2/m_{with strain rate sensitivity}_{m}= 0.5. Further, they

proposed a viscoplastic material model consistent with these observations. This

was later analyzed in detail by Molinari and Ravichandran [58] using the model

proposed by Clifton [19].

The analysis and the models developed in [58] and [75] work very well under the assumption of homogeneous materials. However, in a heterogeneous material, the

propagating waves will undergo scattering due to internal reflections, which leads

to energy dissipation. Grady [35] studied the fundamental questions of entropy

production and basis of stress differences between the Hugoniot and the Rayleigh line

in a structured wave. The phenomenon of scattering in heterogeneous materials was

offered as an alternate explanation to the formation of structured waves. The acoustic

scattering of a finite amplitude shock wave was studied by arguing that the energy

was a combination of lattice strain energy and a vibrational energy. The vibrational

(a)

(b)

Figure 2.6: (a) Shock waves are idealized as moving discontinuity. However, a smooth, structured profile is observed (depicted in bold red) in experiments. The shock is preceded by an elastic precursor traveling at speedUe. (b) Modifiedσ−

Hugoniot curve to depict the Hugoniot Elastic Limit (HEL). The response is linear tillσH E Lis achieved.

stress. Using a phonon relaxation model inspired by statistical thermodynamics,

anelastic equations were formulated that were consistent with phenomenological

equations for structured waves developed in earlier studies [12]. While the model

readily described the single-shock data for metals, it did not work very well for

two-step shocks.

Figure 2.7: Schematic of the experimental setup used by Zhuang [89]. Particle velocity profiles were captured for different combination of impact speeds, layer thickness, material, layer arrangement and number of layers.

conducted on periodically layered composites by Zhuang [89]. Figure 2.7 shows the

schematic of the experimental setup. The target composite was made of alternate

layers of hard and soft materials. Particle velocity profiles were captured using a

VISAR setup. It was observed that the shock structure is significantly influenced by

the material heterogeneity. Factors like loading amplitude, impedance mismatch,

number of layers, propagation distance and pulse duration were explored. It was

observed that the shock front steepens with increase in loading amplitude. Figure 2.8a shows the difference in particle velocity profiles upon change of impedance

mismatch between the composite layers. The shock steepens upon decrease in

impedance mismatch indicating better wave transmission. Figure 2.8b shows the

dependence of particle velocity profile on number of interfaces, keeping the total

target thickness constant. The steepening of the shock front with the increase in

number of interfaces was attributed to the increasing nonlinearity of the system.

A scaling law ˙ = β(∆σ)nwas also calculated and it was observed thatn≈1.8−2.4

instead of 4, as observed by Swegle and Grady [75]. This was purely the effect of heterogeneity, as the individual component materials hadn ≈4. Physically it means that the shock viscosity increases due to the wave scattering in the presence of

heterogeneities. The fourth power law was further investigated by Grady [36]. It

was shown that invariance of the energy-time product is a more fundamental notion

from which the fourth power law can be recovered in the case of steady shock waves.

A few studies on composites and porous solids were also reported where the fourth

(a)

(b)

Figure 2.9: Schematic of the experimental setup used by Rauls [65]. A powder gun accelerates an Aluminum impact to impact a two phase composite specimen. Measurements were done using PDV at the right end of the target.

and the associated shock viscosity was not addressed, and it still remains an open

problem.

Vogler [79] conducted numerical simulations to study the scaling laws in

hetero-geneous materials for three types of materials - layered composites, particulate

composites and granular materials. In case of layered materials, the simulations

agreed with experimental observations of Zhuang [89] and a second power law

scal-ing was recovered. In case of particulate composites, a scalscal-ing power of 2−3 was recovered. It was pointed out that scattering associated with the particulate nature

of the composite played a significant role in the reduction of scaling power. In the

case of granular materials, a linear scaling law was observed. A separate model,

taking into account the pore collapse, was proposed to explain the linear scaling.

Recently, plate impact experiments were conducted by Rauls [65] on two phase

composites. Figure 2.9 shows the schematic of the experimental setup. The target

used was a two phase composite made of PMMA matrix with glass beads as

inclu-sions. Figure 2.10 shows the cross section of the composite sample. The horizontal

markings on the cross section came from polishing the sample for imaging.

Par-ticle velocity profiles were measured using Photon Doppler Velocimetry (PDV) at

three points on the target surface. Experiments were carried out for different sizes (100µm, 300µm, 500µm, 700µm and 1000µm) of glass beads and different bead volume fractions (30% and 40%).

Figure 2.10: A cross section of the two phase composite sample used in [65] made from PMMA matrix and glass beads as inclusions

structure. Figures 2.11a and 2.11b show particle velocity profiles for 100µm and 100µm. As the mean bead size increased with fixed volume fraction, the slope of the profile reduced, implying lower shock speeds. Additionally, a structure developed

at the leading edge and near the point of maximum particle velocity implying

larger shock width. The presence of overshoot in the profiles, which occurs due to

secondary reflections, was also a consequence of heterogeneity. Since the volume

fraction was kept fixed, increasing the bead size effectively reduced the number of interfaces. This information was reflected into the decrease of overshoot observed

in the profiles. Shock rise times scaled linearly with bead size for a fixed volume

fraction, with shock width increasing by an order of magnitude between 100µm and 1000µm. CTH simulations showed that for larger bead size, due to the decrease in number of beads and increase in bead spacing, the linear scaling of the shock width

started to break down.

From a theoretical perspective, scattering of elastic waves in a periodic medium has been studied extensively. In a periodic medium using Bloch-floquet theory,

frequency responses have been studied by Sun [74], Lee and Yang [46] and Nayfeh

[61] among others. Studies have also been conducted for elastic waves in a random

medium by Ryzhik [67] and have showed how scattering results in a diffusive

response. However, very little is known about nonlinear wave propagation in a

heterogeneous medium. Using Bloch-Floquet theory, plate impact response of

periodic laminate was studied by Chen [18]. An approximate solution for the plate

(a)

(b)

Figure 2.11: Particle velocity profiles for bead size (a) 100µm and (b) 1000µm for 40% volume fraction. Profiles are measured at three points of the sample to account for spatial heterogeneity. The profile for 1000µm beads has less steep slope with rounded structures towards the leading and trailing edges of the shock. Additionally, the overshock is greater for the 100µm bead size due to greater number of beads, hence greater number of interfaces, leading to contributions from secondary reflections.

wave solution. An expression for mean stress was derived for moderate shocks and

scattering was accounted for in the form of wave trains. Each wave train had a

then expressed as a combination of mean stress and time dependent contribution

*C h a p t e r 3*

### SHOCK WAVE SCATTERING IN LAYERED MATERIALS

[1] Vinamra Agrawal and Kaushik Bhattacharya. “Shock wave propagation through
a model one dimensional heterogeneous medium”. In:*International Journal*
*of Solids and Structures* 51.21–22 (2014), pp. 3604–3618. issn: 0020-7683.
doi: http : / / dx . doi . org / 10 . 1016 / j . ijsolstr . 2014 . 06 . 021.
url: http : / / www . sciencedirect . com / science / article / pii /
S0020768314002534.

In this chapter, the phenomenon of scattering is analyzed in a layered, not necessarily

periodic, medium. Specifically, a one-dimensional system made of perfectly bonded

homogeneous layers is considered. An overall picture is developed by studying

individual wave interactions in the system.

**3.1** **Problem Description**

Figure 3.1 shows the schematic of the impact problem on the layered composite. The

layers are assumed homogeneous and perfectly bonded to ensure continuity of dis-placements across the material interfaces. As explained in Section 2.3, the material

under shock loading follows a Hugoniot curve represented in Figure 2.6b. While the

loading is governed by a Hugoniot curve, the unloading happens along an isentrope

leading to the formation of rarefaction waves. Unlike shock waves, the states across

rarefaction waves are not discontinuous. Rarefaction waves are represented as a

‘wave-fan’ across which states are connected continuously [23]. These waves are

characteristic of the convex super-linear behavior of the Hugoniot beyond the

Hugo-niot elastic limit. Impact, wave-wave interactions and wave-material interactions

lead to a complex system of shock waves and rarefaction waves into the material. In order to simplify the analysis in this problem, the Hugoniot is approximated by a

piecewise linear stress strain curve as represented in Figure 3.1. In other words, the

rarefaction waves are no longer present in the system as they can be collapsed onto

a single ‘elastic’ wave.

As explained in Section 2.3, shock problems are typically augmented with a linear

Us − v Hugoniot. In this problem, following Knowles [44], the piecewise affine stress-strain relationship is augmented with a kinetic relation that relates shock

introduced by Abeyaratne and Knowles [1], [4] to study phase transitions. However,

it has been useful to study shock wave propagation ([44], [62]). Further, the structure of the shock is neglected in this analysis. This means that the shock is assumed to

be a moving discontinuity. This is because the kinetic relation can be chosen in such

a way that dissipation at the discontinuity and the dissipation due to the structured

shock is equal [4]. Additionally, in a more recent study by Tan [76], it was shown

that sharp front assumption is valid if the length scale of the heterogeneity is much

larger than the inherent shock width.

Figure 3.1: Schematic representation of plate impact

The problem setup (Figure 3.1) shows a layered composite consisting of N layers, ρiandLibeing the density and thickness of theit h layer, being impacted upon by a linear elastic flyer traveling at speedvimpact. The left edge of the flyer and the right edge of the layered composite has a traction free boundary condition. For now, the

piecewise affine stress-strain curve is parameterized by three quantities - yield stress σ1, the modulusE, and the compliant strainεC. Additionally, every layer is assumed

to have the same ρ, σ1andE. The case with relaxed assumption will be addressed

later. This assumption simplifies the analysis by reducing the heterogeneity to

shock waves and making the composite homogeneous to elastic waves. This will be

addressed in detail in Section 3.2. Finally, the system is assumed isothermal.

**3.2** **Governing equations**

The problem is formulated in Lagrangian setting with X = 0 being on the left

and particle velocity at any point X at time t is denoted by σ(X,t), ε(X,t) and v(X,t), respectively. The compressive stresses and strain are taken to be positive as notation. The system is governed by the set of compatibility and conservation

laws as presented in Section 2.1. Additionally, due to the isothermal assumption,

conservation of energy is not required as it is automatically taken care of by the

kinetic relation and the dissipation inequality. The piecewise affine stress-strain

curve allows the system of equations to reduce to following jump equations:

~σ+ ρs˙~v= 0, (3.1)

~v+s˙~ε= 0, (3.2)

where ˙sis the speed of the propagating discontinuity.

An*elastic*wave is described as a moving discontinuity across which the states lie

in the same branch of the stress-strain curve. Further, a*shock*wave is characterized

by the moving discontinuity across which the states lie on different branches of the stress-strain curve. This is represented in Figure 3.2a, where states 1-2 and Q-3 are

connected through an elastic wave and states 2-3 are connected by a shock wave.

For an elastic wave, it can be shown that the equations (3.1) and (3.2) hold if and

only if,

˙

s= ±c =± s

E

ρ. (3.3)

The assumption of uniform ρ, E and σ1 allows the same elastic wave speed c

for all layers, thereby making the system homogeneous to elastic waves. The

heterogeneity is only limited to shock waves. The dissipation across the shock front

can be represented as the signed area between the line 2−3 and the stress strain curve between the points 2 and 3. This means that across the shock front, the dissipation

is given by the difference in areaP3QandP21.

For this analysis, a*maximally dissipative*kinetic relation [83] is used as the additional

empirical law to complete the set of equations to obtain a unique solution. Physically,

it means that the shock tries to maximize the dissipation [62]. Maximal dissipation

kinetics is thermodynamical equivalent of the Lax entropy criteria [47] widely used

in shock physics. Thus, for a compression shock taking the material from the low-strain branch to the high-low-strain branch, the low low-strain state has to coincide with

point 1 for maximal dissipation kinetics to be satisfied. Along the same lines, the

tensile shock from high-strain branch to low-strain branch can satisfy the maximal

(a)

0 0.1 0.2

0 0.2 0.4

v/c →

U/c

→

(b)

(a)

(b)

Figure 3.3: (a)X−t diagram for the shock interaction problem at the A-B material interface. The impinging shockUA interacts with the material interface to produce the elastic waves and a shockUB.

3.2a. A formal expression of the kinetic relation can also be derived using the jump

equations (3.1) and (3.2) as follows:

−_{~}v_{}= Uc

2_{εc}

c2_{−}_{U}2. (3.4)

The expression (3.4) for the kinetic relation is represented in Figure 3.2b. Although

this is not a linear expression, a linear approximation can be made for a large range

of under-driven shocks.

**3.3** **Shock wave interaction at a material interface**

In this section, the fundamental problem of the interaction of a shock wave at

interface, are considered with initial stress-free configuration. A sudden loading σ0> σ1is applied to the left end and the resulting wave problem is studied. Figures

3.3a and 3.3b show theX−tdiagram of the problem and the equivalent representation in the stress-strain space, respectively. The loading produces a combination of an

elastic wave and a shock wave into the material A. Since the system is homogeneous

to elastic waves, the elastic wave propagates unimpeded into the material B. In

order to satisfy the maximal dissipation kinetics, the elastic wave needs to take the

material from unstressed configuration to point 1 in the stress strain curve shown in

Figure 3.3b. The shockUA takes the state of the material A from point 1 to 2, with σ2= σ0as shown in Figure 3.3b. The jump equations across the elastic and shock

waves are given by

σ1−0+ ρc(v1−0)= 0, (3.5)

σ2−σ1+ ρUA(v2−v1)= 0, (3.6)

v2−v1+UA(ε2−ε1)= 0. (3.7)

Since the statesσ1, σ2,ε1andε2are known, the above equations can be solved for

v1, v2andUA to give

v1= −

σ1

ρc, (3.8)

UA=

r σ

2−σ1

ρ(ε2−ε1)

, (3.9)

v2= v1− p

ρ(σ2−σ1)(ε2−ε1). (3.10)

Upon interaction of the shock wave at the A-B material interface, following waves

can potentially form as shown in Figure 3.3a:

1. An elastic wave originating from the point of interaction propagating back

into A taking the state of A from point 2 to 3.

2. An elastic wave propagating into B taking the state of B from point 1 to 4.

3. A shock wave propagating into B taking the state of B from 4 to 5.

From the previous discussion, the maximal dissipation kinetics enforces state 4 to

coincide with 1. More precisely,σ4 =σ1, givingv4= v1. Physically this means that

the forward propagating elastic wave B will not exist in the system. Additionally,

only state 3 needs to be determined. Writing jump equations across the elastic wave

in A and across the shock wave in B,

σ3−σ2− ρc(v3−v2) =0, (3.11)

σ2−σ1+ ρUB(v2−v1=0, (3.12)

v3−v1+UB(ε3−ε1) =0. (3.13)

Solving these equations give,

σ3=

EεB

cσ1−σ2_{1}+(σ2+ ρc(v1−v2))2

2(σ2−σ1)+ ρc(εBcc+2v1−2v2)

, (3.14)

v3=

(EεB_{c}(σ1−σ2+ ρcv2))−(σ1−σ2+ ρc(−v1+v2))(σ1−σ2+ ρc(v1+v2))

ρc(−2σ_{1}+2σ_{2}+ ρc(εBcc+2v1−2v2))

, (3.15)

UB = σ2−σ1+ ρc(v1−v2) σ2−σ1+ ρc(εBcc+v1−v2)

. (3.16)

Simplification of above expressions results in

UB = rUAc

c+(r−1)UA, (3.17)

wherer =ε_{c}A/εB_{c} is the compliance ratio between the two materials. It can be seen
from (3.17) that ifr < 1, which means that the shock passes from a less compliant
to a more compliant medium, the shock speed decreases. Similarly, if r > 1, the
shock speed increases. A similar expression for σ3, purely in terms of r, cannot

be derived becauseσ3can not be eliminated. Second, the forward moving elastic

wave in B is not present in this system, which is a consequence of the kinetic law.

Finally, the receding elastic wave in B eventually brings the entire laminate to the

same stress stateσ3.

In the analysis involving a Hugoniot, instead of a piecewise affine relation, the

**3.4** **Semi-infinite medium**

In order to get one step closer to the problem in Figure 3.1, a laminate with N

segments is chosen. The impactor and the last layer of the laminate are assumed

to be semi-infinite. This assumption removes any possible wave reflections from

the ends of the target or the impactor. Additionally, as pointed out in the earlier

section, the laminate is homogeneous to elastic waves and the interaction of a shock at material interface does not produce any forward propagating elastic waves. This

implies that the shock never interacts with an elastic wave and the only interaction

is that with a material interface. As such, the problem can be described exactly as

in the previous section. The shock speed in the Nt h layer can be expressed as

UN = rNU1c c+(rN −1)U1

, (3.18)

whererN = ε1_{c}/ε_{c}N is the ratio of compliant strain of the first and the last layer.
The expression (3.18) implies that the speed of the shock in the semi-infinite medium

depends only on the properties of the first and the last layer. The properties and the

arrangement of intermediate layers in this model do not play a role in determining

the final state. Again, the receding elastic waves will eventually bring the entire

system to the common stress stateσN.

**3.5** **Finite heterogeneous medium: Method**

In this section, the semi-infinite assumption is removed from the previous section.

This adds a lot more complexity in the system due to the elastic waves reflecting

off the free surface and interacting with the shock. It is important to note that the

solution(v, σ)is piecewise constant due to the nature of the stress-stress curve. This

means that following the waves is enough to generate the solution. The numerical

scheme presented in the next section follows every elastic wave and shock wave as

it nucleates and propagates into the system. As a first step, all possible interactions

between waves and interfaces are cataloged. These interactions are posed locally as

Riemann problems with piecewise constant initial data.

**Individual interactions**

An advantage of having a piecewise linear stress-strain curve is that the all possible interactions can be classified into the following classes of Riemann problems.

1. Reflection of an elastic wave from a free edge

a) Interaction within a linear elastic material

b) Interaction within a piecewise affine material

i. Interaction resulting in the formation of two elastic waves

ii. Interaction of waves in low-strain branch forming a pair of com-pression shocks

iii. Interaction of waves in high-strain branch forming a pair of tensile shocks

c) Interaction at the interface of linear and piecewise affine material

i. Interaction resulting in the formation of two elastic waves

ii. Interaction resulting in the formation of a compression shock in

piecewise affine material

iii. Interaction resulting in the formation of a tensile shock in piecewise

affine material

3. Elastic wave in piecewise affine material crossing material boundary to enter

another layer

4. Elastic wave from a linear elastic material entering a piecewise affine material

a) Interaction forming a compression shock in piecewise affine material

b) Interaction forming a tensile shock in piecewise affine material

c) Low amplitude wave passing through unimpeded

5. Interaction of a compression shock at an interface

a) Interface connects a linear elastic and piecewise affine material

b) Interface connects two piecewise affine materials

6. Interaction of a tensile shock at an interface

a) Interface connects a linear elastic and piecewise affine material

b) Interface connects two piecewise affine materials

7. Interaction of a shock wave with an elastic wave

a) Compression shock and elastic wave traveling in the same direction

b) Compression shock and elastic wave traveling in the opposite direction

d) Tensile shock and elastic wave traveling in the opposite direction

8. Interaction of two shock waves traveling in opposite direction

a) Compression shocks

b) Tensile shocks

**Solutions to Riemann problems**

Following the procedure listed in Section 3.3, explicit solutions to a few Riemann

problems mentioned above are derived in this section.

**Interface interactions**

a. Elastic wave from a purely elastic medium entering a piecewise affine medium:

Figures 3.4a and 3.4b show the schematic of such an interaction. As shown in Figure 3.4b, material A is purely elastic while material B is piecewise linear. Depending

upon the states a and b in Figure 3.4a, there are three possible cases.

(a) (b)

Figure 3.4: Schematic diagram of the elastic wave interaction at A-B interface

*Case 1: No shock formation: This happens when either* σa < σ1, σb ≤ σ1 or

σa > σ1, σb ≥ σ1. Since the layers are elastically homogeneous, in this case the

elastic wave passes through the interface without any interruption.

*Case 2: Formation of compression shock: Figure 3.5a shows the case when the*
interaction leads to the formation of compression shock. This happens whenσa ≤

σ1and σb > σ1. In case σa = σ1, the state just ahead of the point of interaction

needs to be considered to decide if case 1 is applicable or case 2. The process in

stress-strain space is represented in Figure 3.5b. The maximal dissipation criteria

given by

U = c(−2σ1+σa+σb+cρ(va−vb))

−2σ_{1}+σa+σb+cρ(εcc+va−vb).

(a) (b)

Figure 3.5: Elastic wave interaction leading to a compression shock

*Case 3: Formation of unloading shock: Figure 3.6a shows the formation of an*

unloading shock during this interaction. This happens whenσa ≥ σ_{1}andσb < σ1.

Just as in case 2, if σa = σ1, the state ahead of the point of interaction needs to

be considered to decide if case 1 is applicable or case 3. The Riemann problem in

stress-strain space is presented in Figure 3.6b. Finally, the shock speed is given by

U =c− Eεcc

2σ1−σa−σb+ ρc(εcc−va+vb)

.

It should be noted that state d in Figure 3.6a can be of unloading nature which can

lead to the separation of A-B interface. This enables the study of spallation and

re-compression shocks.

(a) (b)

Figure 3.6: Elastic wave interaction leading to an unloading shock

b. Compression/Unloading shock entering a purely elastic medium: The

Section 3.3. The case of a shock wave interacting with the interface of a nonlinear

and linear material is considered here. Figures 3.7a and 3.7b show the Riemann problem of a compression shock interacting with the interface of nonlinear and

linear material in X −t and stress-strain space, respectively. The interaction leads to the formation of two elastic waves. The state d in Figure 3.7a and 3.7b is given

by

σd = 1

2 σ1+σb+ ρc(va−vb)

,

vd = 1

2ρc σ1−σb+ ρc(va+vb)

.

(a) (b)

Figure 3.7: Compression shock wave entering a purely elastic material

The case of unloading shock is represented in Figures 3.8a and 3.8b. The state d in

Figures 3.8a and 3.8b can be calculated from the same expressions above.

(a) (b)

Figure 3.8: Compression shock wave entering a purely elastic material

c. Unloading shock entering another nonlinear material The interaction of an

un-loading shock at the interface of two nonlinear layers leads to the formation of